Syntheses, Structure, and Selected Physical Properties of CsLnMnSe3 (Ln = Sm, Gd, Tb, Dy, Ho, Er, Tm, Yb, Y) and AYbZnQ3 (A = Rb, Cs; Q = S, Se, Te)
Kwasi Mitchell; Fu Qiang Huang; El'ad N. Caspi; Adam D. McFarland; Christy L. Haynes; Rebecca C. Somers; James D. Jorgensen; Richard P. Van Duyne; James A. Ibers; Inorganic Chemistry 43 (2004) 1082–1089; doi:10.1021/ic030232+

data_4327363
_publ_section_title
;
 Syntheses, Structure, and Selected Physical Properties of CsLnMnSe3 (Ln =
 Sm, Gd, Tb, Dy, Ho, Er, Tm, Yb, Y) and AYbZnQ3 (A = Rb, Cs; Q = S, Se,
 Te)
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1082
_journal_page_last               1089
_journal_paper_doi               10.1021/ic030232+
_journal_volume                  43
_journal_year                    2004
_chemical_formula_sum            'Cs Mn Se3 Sm'
_chemical_formula_weight         575.08
_chemical_name_systematic
;
  ?
;
_space_group_IT_number           63
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   4.2618(7)
_cell_length_b                   15.715(3)
_cell_length_c                   11.2232(19)
_cell_measurement_temperature    153(2)
_cell_volume                     751.7(2)
_computing_cell_refinement       'SMART version 5.054 (Bruker, 2000)'
_computing_data_collection       'SMART version 5.054 (Bruker, 2000)'
_computing_data_reduction        'SAINT-Plus version 6.22 (Bruker, 2000)'
_computing_molecular_graphics    'SHELXTL-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXTL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      153(2)
_diffrn_measured_fraction_theta_full 0.967
_diffrn_measured_fraction_theta_max 0.967
_diffrn_measurement_device_type  'Bruker Smart 1000 CCD'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0311
_diffrn_reflns_av_sigmaI/netI    0.0167
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            4560
_diffrn_reflns_theta_full        28.89
_diffrn_reflns_theta_max         28.89
_diffrn_reflns_theta_min         2.59
_diffrn_standards_decay_%        <2
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    28.592
_exptl_absorpt_correction_T_max  0.56470
_exptl_absorpt_correction_T_min  0.11217
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'faces indexed'
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    5.082
_exptl_crystal_description       needle
_exptl_crystal_F_000             976
_exptl_crystal_size_max          0.184
_exptl_crystal_size_mid          0.066
_exptl_crystal_size_min          0.020
_refine_diff_density_max         1.860
_refine_diff_density_min         -1.326
_refine_diff_density_rms         0.372
_refine_ls_extinction_coef       0.00185(14)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.981
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     24
_refine_ls_number_reflns         565
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.981
_refine_ls_R_factor_all          0.0184
_refine_ls_R_factor_gt           0.0177
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
; calc
  [1.00000+0.00000exp(0.00(sin\q/\l)^2^)]/
    [\s^2^(Fo^2^)+0.0000+0.0000*P+(0.0400P)^2^+0.0000sin\q/\l]
  where P = 1.00000Fo^2^ + 0.00000Fc^2^
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0481
_refine_ls_wR_factor_ref         0.0486
_reflns_number_gt                544
_reflns_number_total             565
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic0302322B_1.cif
_cod_data_source_block           CsSmMnSe3
_cod_database_code               4327363